International Desalination Association BAH03-102 1
THE SELECTION DESIGN, FABRICATION AND PERFORMANCE OFZERON100 IN SWRO APPLICATIONS.
Authors G Byrne, R Francis, G Warburton. R.J Bullock & C Kuzler1
Presenter: G Byrne
Super Duplex Stainless Steels (SDSS) are finding increasing use in high pressure feed pipework systemson SWRO plants and in other desalting applications using membrane technology.
This paper details the corrosion resistance of ZERON 100 SDSS in seawater service, comparing andcontrasting this with other grades of steel commonly used in SWRO applications.
Key aspects of product design that allow for the construction of lower cost, more mechanically efficientpipework systems and vessels are detailed. Again these are compared and contrasted with other steelsused in SWRO plants.
Fabrication practices and procedures are discussed and welding, forming, machining and galvaniccompatibility with other steels are considered.
Specific case studies are presented where ZERON 100 SDSS has been successfully used in small scaleand large scale new build SWRO applications.
Also presented are cases where the alloy has been successfully used to replace SWRO pipeworkconstructed in other grades of stainless steel that have suffered corrosion failure in service.
Finally the successful use of the steel in novel membrane systems on offshore platforms is alsopresented.
International Desalination Association BAH03-102 2
This paper considers the nature of the alloy chemistry of ZERON 100, its microstructure and theresultant properties that make it attractive to the design engineer for Sea Water Reverse Osmosis(SWRO) applications. Aspects of design and fabrication to optimise its commercial attraction andperformance in service are also detailed.
II. CORROSION RESISTANCE
The diversity of stainless steel grades, the variation in costs and contradictory reports of their resistanceto corrosion in seawater make it difficult for design engineers to establish a settled and undisputedmaterial philosophy. All stainless steels rely for corrosion resistance upon the formation of a Chromiumrich, oxide film on their surface, known as a passive film. Other elements, in particular molybdenum,nitrogen and tungsten are known to make the passive film, more difficult to breakdown in the presenceof the chloride ion. Figure 1 shows that the passive film in most stainless steels is stable over a widerange of potentials. It also shows what elements extend this range of passivity or enhance corrosionresistance . It can be seen that passivity is lost under highly oxidising (transpassive) conditions andwhen active, general corrosion occurs. Increased temperature also has a negative effect on passivity.
F IG U R E 1 S c h e m a tic d ia g ra m s h o w in g th ee ffe c ts o f a l lo y in g e le m e n ts o n th e
c o r ro s io n o f s ta in le s s s te e ls
C u rre n t D e n s ity / C o rro s io n
A c tiv e
T ra n s p a s s iv e C r , M o , N , W
C rC r , N i, M o
C r , N i, W
International Desalination Association BAH03-102 3
A convenient, yet empirical, point of entry to differentiate between the corrosion resistance of stainlesssteels in chloride environments has been provided by Truman . Using linear regression analysis ofchemical composition and pitting and crevice corrosion test data, Truman identified a strong correlationbetween a parameter known as the Pitting Resistance Equivalent (PREN) and, both the critical pittingand critical crevicing temperature (CPT/CCT) for a wide range of stainless steels in chloride solution(Figure 2).
The validity of this relationship has been confirmed by many subsequent authors. Kovach and Redmond published an excellent review of the history of this work, rationalizing differences and discrepanciesin test technique, alloy chemistry and seawater conditions and drawing compelling conclusions as to therelationship between PREN and CCT in seawater. By comparing the results of long term crevicecorrosion tests in warm seawater with laboratory results from ASTM G48 Method D corrosion tests,these authors found that only those alloys with a CCT of 35C or higher in the Method D test resistedcrevice corrosion in warm seawater (Figure 3).
FIGURE 2 Critical pitting temperatureversus PREN for some stainless steels
20 25 30 35 40 45 50
PREN (%Cr + 3.3%Mo + 16%N)
FIG UR E 3 P ercen tag e of sites a ttacked vscritica l crevice tem perature in AS TM G 48D
(K ovach e t a l)
0 10 2 0 30 40 50 60
C C T A S TM G 48D (C )
Ferrit ic Au sten itic D up lex
International Desalination Association BAH03-102 4
Further, they were able to relate this behavior to the PREN number of a range of stainless steels anddetermine the PREN level necessary to avoid crevice corrosion (Figure 4).
This means that for seawater service only SDSS with a PREN of 40 minimum and super austeniticstainless steels (SASS) grades with a PREN of 45 minimum should be considered if crevice corrosion isto be avoided. However, this considers only seawater with typical chloride contents of 18-20,000 ppm.On brine rejection circuits this figure may double and we understand developments in membranetechnology may further concentrate the reject brine with chloride. Figure 5 shows that under mildlyoxidising conditions the CPT of Zeron 100 welds remains at about 50C as the chloride contentincreases from 20,000 mg/l to 100,000 mg/l. The crevice corrosion resistance was displaced to evenhigher temperatures as the chloride content was reduced correspondingly.
Figure 4 Relationship Between PREN andCritical Crevice Temperature (ASTM G48D)
0 10 20 30 40 50 60
PREN (%Cr + 3.3%Mo + 16%N)
FIGURE 5 CCT/ CPT versus chlorideconcentration at a potential of +400mV SCE
0 20 40 60 80 100 120
CCT/ CPT (C)
CCT (Parent) CPT (Weld)
International Desalination Association BAH03-102 5
The performance of high alloy stainless steels and nickel alloys in seawater service is dependent upontheir proper chemical formulation, processing, heat-treatment and finishing.
The proper combination of alloy chemistry and thermo-mechanical processing is of prime importance.However, Shone  also found that:-
2.1 Poor pickling was leading to crevice corrosion of alloy 625 that had previously been believed tobe immune to crevice corrosion in seawater. Grubb  confirmed the significance of picklingwith respect to 6% Molybdenum alloys similarly .
2.2 Variation in performance between plate and tube products in 6% Molybdenum alloys wasattributable to differences in processing.
2.3 Small differences in alloy chemistry of duplex and austenitic grades was giving rise todifferences in crevice corrosion resistance.
In view of this, designers and specifiers should seek a consistency in supply source of the raw material(bar, billet, plate and seamless pipes). They should ensure all converters of raw material to finished andsemi finished products are approved and qualified to manufacture by the supplier of the steel. Thisshould ensure that all thermo-mechanical processing of the material is compatible with the basechemistry of the raw material provided. Without this level of consistency in material, variation inperformance can arise . Most reputable steel companies dealing with branded alloys appreciate thisand work hard to retain brand integrity across all product forms.
So, purchase specifications should require tests confirming a suitable level of performance. Theseusually involve ASTM G48 Method A corrosion tests, Charpy impact tests and microstructure tests.This approach has been standardized in the form of ASTM A923. However, the scope of this standard islimited to the detection of intermetallics and does not address fitness for purpose.
Table 1 shows the composition and mechanical strength of a range of stainless steels used in SWROplants.
NOMINAL COMPOSITION (WT%)ALLOY Fe Cr Ni Mo Cu W N PREN
316L bal 17 10 2 - - - 24 170 485
904L bal 20 25 4.5 1 - - 35 215 490
6Mo Aust. bal 20 18 6 0.7 - 0.2 43 300 650
bal 25 7 3.5 0.7 0.7 0.25 >40 550 750
bal 25 8 3.5 0.7 0.7 0.25 >40 450 700
International Desalination Association BAH03-102 6
Figure 6 plots the relative localised corrosion resistance as quantified by the PREN number against thestrength level of these steels. From this it can be seen that the family of duplex steels mirrors the familyof austenitic stainless steels in terms of corrosion resistance but with the benefit of 2 x strength and theadded benefit of higher resistance to chloride stress corrosion cracking.
Table 2 shows the allowable stresses for pipework and vessels of SASS and SDSS alloys according toBritish and